MODELLING LONG-TERM EVOLUTION OF CEMENTITIOUS ... MODELLING LONG-TERM EVOLUTION OF CEMENTITIOUS...
Embed Size (px)
Transcript of MODELLING LONG-TERM EVOLUTION OF CEMENTITIOUS ... MODELLING LONG-TERM EVOLUTION OF CEMENTITIOUS...
MODELLING LONG-TERM EVOLUTION OF CEMENTITIOUS MATERIALS USED IN WASTE DISPOSAL
D. JACQUES1*, J. PERKO*, S. SEETHARAM*, D. MALLANTS**, J. GOVAERTS*
*Belgian Nuclear Research Centre (SCK•CEN), Institute for Environment, Health, and Safety, Mol, Belgium.
**CSIRO Land and Water, Waite Road - Gate 4, Glen Osmond SA 5064, Australia.
This report summarizes the latest developments at SCK•CEN in modelling long-term evolution of cementitious materials used as engineered barriers in waste disposal. In a first section chemical degradation of concrete during leaching with rain and soil water types is discussed. The geochemical evolution of concrete thus obtained forms the basis for all further modelling. Next we show how the leaching model is coupled with a reactive transport module to determine leaching of cement minerals under diffusive or advective boundary conditions. The module also contains a simplified microstructural model from which hydraulic and transport properties of concrete may be calculated dynamically. This coupled model is simplified, i.e. abstracted prior to being applied to large-scale concrete structures typical of a near-surface repository. Both the original and simplified models are then used to calculate the evolution of hydraulic, transport, and chemical properties of concrete. Characteristic degradation states of concrete are further linked to distribution ratios that describe sorption onto hardened cement via a linear and reversible sorption process. As concrete degrades and pH drops the distribution ratios are continuously updated. We have thus integrated all major chemical and physical concrete degradation processes into one simulator for a particular scale of interest. Two simulators are used: one that can operate at relatively small spatial scales using all process details and another one which simulates concrete degradation at the scale of the repository but with a simplified cement model representation.
1. MODELLING CHEMICAL DEGRADATION OF CONCRETE DURING LEACHING WITH RAIN AND SOIL WATER TYPES
Cement and concrete are typically not in thermodynamic equilibrium with the surroundings in which they are located. Because concrete used in e.g. waste conditioning and surface disposal is not an isolated system, water infiltration and solute migration from the surrounding environment will alter the concrete pore water and solid phase composition. As a result, the solubility and sorption of contaminants will change too (see Wang et al.  for an extensive review of sorption values for radionuclides and chemically toxic elements as function of the cement degradation state).
While concrete degradation usually occurs as the result of a combination of physical, mechanical, and chemical processes, this paper emphasizes the role of chemical degradation. Typical chemical degradation reactions are decalcification, dissolution and leaching of cement components and carbonation (Glasser et al. ), amongst others. These reactions induce a gradual change in the pore water composition, from typical "young" concrete pore water with a pH above 13 to more evolved pore water with a pH lower than 10. Different attempts have been made to simulate the long term chemical degradation of concrete [3,4,5,6,7]. In general, four states of cement degradation are identified depending on the pH and cement pore water controlling cement phases (pH-values are for the reference temperature of 25°C). State 1 has a pH larger than 12.5 with a high concentration of Na and K ions. State 2 has a pH of 12.5 controlled by the dissolution of portlandite with approximately
1 *Corresponding author: email@example.com
20 mmolal of Ca. State 2 starts when all portlandite has been leached out of the cement and the pH is between 12.5 and 10. The pore water composition is buffered by different cement phases including AFt, AFm and calcium-silicate hydrates (C-S-H phases). The end of this state is defined when all these phases are completely leached out. State 4 has a pH lower than 10 with aggregate minerals present; in this study calcite is the only aggregate used. The pore water composition is then mainly influenced by the composition of the infiltrating water. Although the reactions within each state are quite independent of the composition of the infiltrating water, the duration of the different states and the stoichiometric coefficients of the different dissolution/precipitation reactions depend strongly on the composition of the infiltrating water (see further).
The assessment of the progression of the long-term chemical degradation of cement is possible by means of model simulation. The most straightforward way is using thermodynamic equilibrium modelling coupled with transport of solution species. Such modelling approach is able to reproduce the zoning of cement degradation, as is shown by e.g. Moranville et al. . A more simple approach is to use only thermodynamic equilibrium modelling with a mass balance approach in which, after the equilibrium calculation, the cement-equilibrated pore water is replaced with a new amount of the external aggressive water while keeping the changed cement solid phase. Such type of simulation allows an in-depth analysis of the geochemical changes in both the pore water and the solid phase.
This paper first describes simulations of chemical concrete degradation using thermodynamic equilibrium modelling combined with a mass balance approach for different rain and soil water types accounting for processes as wet deposition, dry deposition, soil biological processes and soil weathering and release of base cations from soils in contact with concrete at ambient surface temperatures (long-term mean temperature of 10°C) using a consistent thermodynamic model for cement phases at temperatures different from the standard temperature (25°C). These calculations were done within the framework of near-surface disposal of low and intermediate-level short-lived radioactive waste in Belgium and coordinated by ONDRAF/NIRAS (Belgian Agency for Radioactive Waste and Enriched Fissile Materials). Atmospheric boundary conditions relevant for determining rain water and soil water composition were taken from nearby meteorological stations. In a second step the mineralogical changes are linked to microstructural changes that determine the pore structure (tortuosity), porosity, hydraulic and transport properties (section 2). A simplified version of this dynamic coupled degradation model is then applied to simulate the degradation of large-scale concrete components of the surface repository (section 3).
1.2. Modelling approach
Chemical degradation of concrete is simulated using mass conservation and thermodynamic equilibrium laws (mass action equations) starting from 1000 cm³ of concrete at a long-term averaged atmospheric temperature (~10°C, representative for Belgium, Jacques and Mallants ). The concrete is equilibrated with a given amount of external water (not in equilibrium with the concrete phases). After equilibration, the resulting water is replaced by a new amount of external water whereas the changed cement solid phase is maintained. In this way, the changing cement pore water and solid phase composition is simulated as function of cumulative added (external) water. This approach needs (i) a consistent thermodynamic database for aqueous species and cement phases for 10°C, (ii) the initial concrete composition and (iii) the composition of the external (soil) water types.
1.2.1. Thermodynamic model for cement degradation
A thermodynamic data set for cement minerals was built by Lothenbach and Winnefeld , Lothenbach et al.  and Matschei et al.  consistent with the thermodynamic data in the Nagra/PSI-Thermodynamic Data Base . When used in the geochemical GEMS-software , temperature dependences of thermodynamic parameters are calculated with the embedded SUPCRT code . The GEMS-software minimizes the Gibbs free energy of the system subject to a number of constraints (mass balance conditions, electrical neutrality). However, the database is not consistent if it is used at temperatures different from 25°C in geochemical codes as PHREEQC  in which geochemical equilibrium is calculated based on mass action equations. To simulate the chemical
degradation due to leaching at a long-term average of the atmospheric temperature (taken to be 10°C in Belgium), the mass action constants of all aqueous species and minerals in the model must be recalculated for this temperature. The Gibbs free energy for all species was calculated with GEMS (based on the revised Helgeson-Kirkham-Flowers equations for aqueous species or the integration of the heat capacity function Cp(T) for minerals and gases) and related to the mass action constant KT by:
KT T rΔexp (1)
where R is the universal gas constant, and ∆rGT° is the Gibbs free energy change of a reaction at temperature T:
Aji iGνG ,Tfr ΔΔ T (2)
where ΔfGT°,Ai is the Gibbs free energy of formation of species Ai at temperature T and vji are the stoichiometric coefficients of the chemical reaction. A detailed description of the conversion of the GEMS-database to a PHREEQC-database, a list of the aqueous species and minerals in the thermodynamic model and corresponding mass action constants at 10°C are given in Jacques 2. Note that the solubility of Na and K in state 1 were slightly dif